Selective Removal of Cs+, Sr2+, and Ni2+by K2xMgxSn3‒xS6(x= 0.5‒1) (KMS-2) Relevant to Nuclear Waste Remediation
Mertz, Joshua L.; Fard, Zohreh Hassanzadeh; Malliakas, Christos D.; Manos, Manolis J.; Kanatzidis, Mercouri G.; Chemistry of Materials 25 (2013) 2116–; doi:10.1021/cm400699r

data_4001778
_publ_section_title
;
 Selective Removal of Cs+, Sr2+, and Ni2+by K2xMgxSn3--xS6(x= 0.5--1)
 (KMS-2) Relevant to Nuclear Waste Remediation
;
_journal_issue                   10
_journal_name_full               'Chemistry of Materials'
_journal_page_first              2116
_journal_paper_doi               10.1021/cm400699r
_journal_volume                  25
_journal_year                    2013
_chemical_formula_sum            'K1.316 Mg0.658 S4 Sn1.342'
_chemical_formula_weight         355
_chemical_name_systematic        ' ?'
_space_group_IT_number           194
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   3.6749(4)
_cell_length_b                   3.6749(4)
_cell_length_c                   16.827(4)
_cell_measurement_temperature    293
_cell_volume                     196.80(6)
_computing_cell_refinement       SAINT
_computing_data_collection       APEX2
_computing_data_reduction        SAINT
_diffrn_ambient_temperature      293
_diffrn_detector                 CCD
_diffrn_detector_type            Bruker
_diffrn_measured_fraction_theta_full 0.98
_diffrn_measured_fraction_theta_max 0.98
_diffrn_measurement_device       'four-cycle diffractometer'
_diffrn_measurement_device_type  'Bruker CCD'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.4428
_diffrn_reflns_av_R_equivalents  0.072
_diffrn_reflns_av_sigmaI/netI    0.0191
_diffrn_reflns_limit_h_max       4
_diffrn_reflns_limit_h_min       -4
_diffrn_reflns_limit_k_max       3
_diffrn_reflns_limit_k_min       -3
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            3198
_diffrn_reflns_theta_full        15.27
_diffrn_reflns_theta_max         15.27
_diffrn_reflns_theta_min         3.02
_diffrn_source                   synchrotron
_exptl_absorpt_coefficient_mu    1.584
_exptl_crystal_density_diffrn    2.9943
_exptl_crystal_F_000             164
_refine_diff_density_max         1.55
_refine_diff_density_min         -1.62
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_gt    2.51
_refine_ls_goodness_of_fit_ref   2.40
_refine_ls_number_constraints    6
_refine_ls_number_parameters     10
_refine_ls_number_reflns         96
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0557
_refine_ls_R_factor_gt           0.0437
_refine_ls_shift/su_max          0.0303
_refine_ls_shift/su_mean         0.0118
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     w=1/(\s^2^(I)+0.0016I^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.1198
_refine_ls_wR_factor_ref         0.1230
_reflns_number_gt                85
_reflns_number_total             96
_reflns_threshold_expression     I>2\s(I)
_cod_data_source_file            cm400699r_si_001.cif
_cod_data_source_block           I
_cod_original_cell_volume        196.81(5)
_cod_original_sg_symbol_Hall     '-P 6c;-2c'
_cod_database_code               4001778